FLEXURAL BEHAVIOUR OF HIGH STRENGTH STEEL
FIBRE NORMAL AND LIGHTWEIGHT CONCRETE BEAMS
©Mohamed Abdulhakim Zurgani, B.Sc.
A thesis submitted to the School of Graduate Studies
in partial fulfillment of the requirement for the degree of Master of Engineering
Faculty of Engineering & Applied Science Memorial University of Newfoundland
An experimental study was conducted to investigate the flexural behaviour of high strength normal and lightweight reinforced concrete beams with steel fibres. Three different mixtures were developed for each type of concrete with three different steel fibre volume ratios. The target compressive strength was 85 MPa. Material and structural experimental programs were performed. In the material investigation, twenty four prisms with dimensions of 100 mm × 100 mm × 400 mm and one hundred and twenty cylinders with dimensions of 100 mm × 200 mm were cast, cured and tested to determine the mechanical properties for all different mixtures. The investigated mechanical properties included the compressive strength, splitting tensile strength, modulus of rupture and flexural toughness.
In the structural investigation, a series of six high strength lightweight aggregate (LWAC) concrete reinforced beams and six high strength normal weight (NWC) reinforced concrete beams were cast and tested. The beams were 200 mm × 400 mm × 3200 mm and were simply supported on a clear span of 2900 mm. The main variables in this study were the concrete type (normal weight concrete and light weight aggregate concrete), steel fibre volume ratio, (0 %, 0.375%, 0.75%), and the longitudinal reinforcement ratio, (0.85%, 1.50%). The structural behaviour of the test beams was examined in terms of load-deflection behaviour, steel reinforcement strain, concrete strain, crack pattern, crack width, crack spacing, mode of failure and ultimate moment capacity.
The test results revealed that the addition of steel fibres to high strength lightweight or normal weight concrete improved the mechanical properties. The compressive strength, splitting tensile strength and the modulus of rupture of fibrous LWAC and NWC concrete increased compared to the plain concrete.
Adding steel fibre to both high strength normal and lightweight concrete increased both cracked and un-cracked stiffness in addition to increasing the ultimate flexural capacity. The steel fibres also enhanced the cracking behaviour for both NWC and LWAC beams, reduced the crack widths and increased the number of the cracks for both type of concrete. The LWAC beams developed more cracks but less cracks width compared to their identical NWC beams. The ductility indexes of fibrous and non-fibrous NWC beams were higher than the ductility indexes measured for the corresponding LWAC beams.
For all fibre reinforced NWC and LWAC beams, CSA A23.3-14, ACI 318-08, EC2-04, and EC2-91 codes overestimated the maximum crack width due to the fact that these models do not consider the presence of steel fibres. The Rilem TC162-TDF was found to accurately predict the maximum crack width of fibrous NWC beams. However, the model was seen to be conservative when predicting the maximum crack width for fibrous LWAC beams.
I am deeply indebted to my thesis supervisor and research advisor Dr. Amgad Hussein, Head of Department of Civil Engineering at Memorial University of Newfoundland; grateful acknowledgment is due for his sincere support, valuable guidance, fruitful discussions, and comments throughout the courses of this study. I would like to thank him for giving me this great opportunity; it was a rewarding experience, both professionally and personally.
I would also like to thank the technical staff at the Civil Department Laboratory, especially Mrs. Shawn organ and Jason Murphy, who helped me a lot, made my work easier, and added pleasant moments in my work. I would also to like all my colleagues who helped me in the lab work.
Finally, my deepest appreciation goes to my family especially my mother for her continuous and unconditional support.
I dedicate this thesis to the memory of my late father; Engineer Abdulhakim Zurgani, who supported and encouraged me throughout his life and passed away while I was writing my thesis; I will miss you so much. You will be in my heart forever.
iii Table of Contents Abstract ... i ... 1 Chapter 1 Introduction ... 1 1.1 General ... 1
1.2 Research Scope and Objectives... 6
1.3 Thesis Outline ... 8
Chapter 2 Literature Review ... 10
2.1 Introduction ... 10
2.2 Previous Experimental Investigations ... 10
2.2.1 Mechanical Properties of Steel fibre Concrete ... 10
2.2.2 Flexural Behaviour of High Strength Reinforced Concrete Beams ... 14
2.2.3 Flexural Behaviour of Normal Strength Steel Fibre Reinforced Concrete beams 15 2.2.4 Flexural Behaviour of High Strength Steel Fibre Reinforced Concrete beams 22 2.2.5 The Flexural Behaviour of Normal Strength Reinforced Lightweight Concrete beams ... 26
2.2.6 The Flexural Behaviour of High Strength Reinforced Lightweight Concrete beams 26 2.2.7 Flexural behaviour of Normal Strength Steel Fibre Reinforced Lightweight Concrete 31 2.2.8 Summary of Experimental Findings in the Literature ... 32
2.3 Codes Provision for Ultimate limit state and Serviceability limit state of Beams. 34 2.3.1 Prediction of Flexural Strength. ... 34
2.3.2 Prediction of Cracking Moment ... 39
2.3.3 Prediction of Crack Spacing ... 42
2.3.5 Summary of Code Equations ... 49
Chapter 3 3.1 Introduction ... 50
3.1.1 Concrete and Aggregates Properties ... 50
3.1.2 Steel Fibres ... 53
3.1.3 Longitudinal Reinforcements ... 54
3.2 Properties of Hardened Concrete ... 54
3.2.1 Compressive Strength ... 54
3.2.2 Splitting Tensile Strength ... 56
3.2.3 Modulus of Elasticity... 57
3.2.4 Modulus of Rupture ... 60
3.2.5 Flexural Load Deflection Curve for Prisms. ... 62
3.2.6 Flexural Toughness ... 65
Chapter 4 4.1 Introduction ... 67
4.2 Test specimens ... 67
4.3 Casting and curing of the Beams ... 70
4.4 Experimental Setup and Instrumentations ... 72
4.5 Test Procedure ... 76
Chapter 5 5.1 Introduction ... 78
5.2 Load Deflection Characteristic... 79
5.3 Ductility ... 90
5.4 Prediction of the Deflection at Service Load ... 95
5.5 Concrete and Reinforcement Strains ... 105
5.6 Cracking Behaviour ... 112
5.6.1 Cracks Patterns ... 112
5.6.2 First Crack Initiation ... 114
5.6.3 Cracking Moment and Codes Predictions ... 117
5.6.5 Codes Prediction for Crack Spacing... 123
5.6.6 Crack Width and Defining Service Load Level. ... 127
5.6.7 Crack Width ... 129
5.6.8 Codes Prediction for Crack Width ... 132
5.7 Moment Capacity ... 136
5.8 Crack Localization... 140
Chapter 6 Summary & Conclusions ... 142
References ... 146
List of Figures
Figure 2.2: Typical Flexural Load-Deflection Curves of Steel Fibre High Strength
Lightweight Concrete. ... 14
Figure 2.1: Stress and Strain Diagram of Fibrous Reinforced Concrete Section. ... 23
Figure 2.3: Strain Distribution and Concrete Stress Block in a Section with Conventional Reinforcement. ... 35
Figure 2.4: Design Assumption for Analysis of Fibrous-Singly Reinforced Beam Proposed by Henager and Doherty in 1976. ... 37
Figure 2.5: Definition for Crack Width Parameters. ... 45
Figure 3.1: Steel Fibres. ... 53
Figure 3.2: The Concrete Compression Testing Machine. ... 55
Figure 3.3: Plain LWAC Concrete Cylinder at Failure. ... 55
Figure 3.4: Splitting Tensile Test Setup. ... 57
Figure 3.5: Modulus of Elasticity Test. ... 58
Figure 3.6: A Photograph of Cylinder During the Modulus of Elasticity Test. ... 58
Figure 3.7: Effect of Steel Fibre Volume Ratio on the Modulus of Elasticity (MPa) of NWC. ... 59
Figure 3.8: Effect of Steel Fibre Volume Ratio on the Modulus of Elasticity (MPa) of LWAC. ... 59
Figure 3.9: Modulus of Rupture Test Machine. ... 61
Figure 3.10: Load vs Deflection Curves for NWC Prisms Specified for Each Beam. ... 62
Figure 3.12: Plain LWAC and NWC Prisms Failure. ... 64
Figure 3.13: Fibrous LWAC and NWC Prisms Failure... 64
Figure 4.1: The Used Wood Formwork and the Steel Frame with =0.85%. ... 70
Figure 4.2: A Photograph During the Casting Process. ... 71
Figure 4.3 : The test Frame. ... 72
Figure 4.4: Strain Gauge Installation on the Steel Bars. ... 73
Figure 4.5: Specimens Details and Strain Gauges Locations. ... 74
Figure 4.6: Strain Gauge Installation on the Beam Compression Side. ... 74
Figure 4.7: Locations of the LVDTs... 75
Figure 4.8: A Photograph during Testing and Crack Marking. ... 77
Figure 5.1: Load Deflection Curve idealization for non-Fibrous Beams. ... 80
Figure 5.2: Load Deflection Curve Idealization for fibrous Beams. ... 80
Figure 5.3: Load vs. Central Deflection for NWC Beams. ... 81
Figure 5.4: Load vs. Central Deflection for LWAC Beams. ... 81
Figure 5.5: Load vs. Central Deflection for NWC and LWAC Beams ... 87
Figure 5.6: Load vs. Central Deflection for NWC and LWAC Beams ... 87
Figure 5.7: Load vs. Central Deflection for NWC and LWAC Beams ... 88
Figure 5.8: Load vs. Central Deflection for NWC and LWAC Beams ... 88
Figure 5.9: Load vs. Central Deflection for NWC and LWAC Beams ... 89
Figure 5.10: Load vs. Central Deflection for NWC and LWAC Beams ... 89
Figure 5.11: Effect of Fibres and the Steel Ratio on the Ductility Measured at the Ultimate Load. ... 94
Figure 5.12: Effect of Fibre and The Steel ratio on The Ductility Measured at The Failure
Load. ... 94
Figure 5.13: Crushing of the Concrete Cover in Beam LB4. ... 94
Figure 5.14: Buckled Compression Reinforcement in Beam LB4. ... 95
Figure 5.15: Load vs Midspan Deflection for Beam NB1. ... 98
Figure 5.16: Load vs Midspan Deflection for Beam NB2. ... 98
Figure 5.17: Load vs Midspan Deflection for Beam NB3. ... 99
Figure 5.18: Load vs Midspan Deflection for Beam NB4. ... 99
Figure 5.19: Load vs Midspan Deflection for Beam NB5. ... 100
Figure 5.20: Load vs Midspan Deflection for Beam NB6. ... 100
Figure 5.21: Load vs Midspan Deflection for Beam LB1. ... 101
Figure 5.22: Load vs Midspan Deflection for Beam LB2. ... 101
Figure 5.23: Load vs Midspan Deflection for Beam LB3. ... 102
Figure 5.24: Load vs Midspan Deflection for Beam LB4. ... 102
Figure 5.25: Load vs Midspan Deflection for Beam LB5. ... 103
Figure 5.26: Load vs Midspan Deflection for Beam LB6. ... 103
Figure 5.27: Load VS. Concrete Strain for NWC Beams with = 0.85%. ... 107
Figure 5.28: Load VS. Concrete Strain for NWC Beams with = 1.50%. ... 107
Figure 5.29: Load VS. Concrete Strain for LWAC Beams with = 0.85%... 108
Figure 5.30 : Load VS. Concrete Strain for LWAC Beams with = 1.50%... 108
Figure 5.31: Load vs. Steel Strain for NWC Beams. ... 111
Figure 5.33: Crack Patterns for NWC Beams at Ultimate Load. ... 116
Figure 5.34: Crack Patterns for LWAC Beams at Ultimate Load... 116
Figure 5.35: Moment vs. Maximum Crack Width for NWC Beams. ... 131
Figure 5.36: Moment vs. Maximum Crack Width for LWAC Beams. ... 131
Figure 5.37: Steel Bar Rupture in Beam NB3. ... 139
Figure 5.38: Beam LB3 at Failure. ... 141
Figure 5.39: Beam NB3 at Failure. ... 141
Figure 5.40: Beam LB6 at Failure. ... 141
List of Tables
Table 3.1: Mixture Proportions For One Cubic Meter of Normal Weight Concrete. ... 52
Table 3.2: Mixture Proportions For One Cubic Meter of Lightweight Aggregate Concrete. ... 52
Table 3.3: Mechanical Properties of the Test Beams. ... 61
Table 3.4: Observed Maximum Load, Displacement at the Maximum Load and Energy Absorption Capacity for NWC Prisms. ... 66
Table 3.5: Observed Maximum load, Displacement at the Maximum Load and Energy Absorption Capacity for LWAC Prisms. ... 66
Table 4.1: Details of Test Beams. ... 69
Table 5.1: Deflection at the First Crack Load, Cracked and Un-Cracked Stiffness Values. ... 84
Table 5.2: Central Deflection Values of The Yielding Load and Ultimate load. ... 86
Table 5.3: Ductility Measurement at Ultimate and Failure Load... 92
Table 5.4: Comparison between the Calculated and Experimental Deflections at Assumed Service Load equal to 0.45 times the ultimate load. ... 105
Table 5.5: Strain in Concrete at Service and Ultimate load. ... 109
Table 5.6: Maximum Crack Depth and Number of Cracks for All Beams. ... 112
Table 5.7: First Cracking Load and Width. ... 115
Table 5.8: Code Recommendations for Modulus of Rupture. ... 118
Table 5.9: Experimental and Code Prediction of Cracking Moments. ... 119
Table 5.11: A Summary of the Equation for Average Crack Spacing. ... 123 Table 5.12: Experimental and Predicted Crack Spacing. ... 126 Table 5.13: The Ratio of the Flexural Reinforcement Stress to Yielding Stress at Different Load Levels. ... 128 Table 5.14: Load Corresponding to 0.3 mm Crack Width and Maximum and Average Crack Width for all Beams. ... 130 Table 5.15: A Summary of Average Crack Width Models... 133 Table 5.16: Comparison of Experimental and Predicted Crack Width for Non-Fibrous Beams... 134 Table 5.17: Comparison of Experimental and Predicted Maximum Crack Width for Fibrous Beams. ... 135 Table 5.18: Comparison between Experimental and Theoretical Moment Capacity Using Reinforcement Stress of fs =fy = 430MPa. ... 138 Table 5.19: Comparison between Experimental and Theoretical Moment Capacity Using Reinforcement Stress of fs=fu= 575MPa... 139
a d Shear span to depth ratio
A Effective tension area, mm2
As Area of the steel reinforcement, mm2
A Minimum area of steel, mm2
b Minimum effective web width, mm
c Depth of the neutral axis, mm
d Effective depth, mm
d Diameter of the steel bar, mm
d Fibre diameter, mm
e Distance from the extreme compression fibre to the top of the tensile stress block of fibrous concrete
E Modulus of elasticity of concrete, MPa
f Concrete compressive strength, MPa
f Characteristic compressive cylinder strength ctm
f Mean value of axial tensile strength of concrete, MPa s
f Stress in the longitudinal reinforcement r
f Modulus of rupture, MPa
f Splitting tensile strength, MPa
f Yield strength of the bars, MPa
F Bond efficiency of steel fibres, MPa m
G Shear modulus of concrete matrix, MPa
h Depth of the beam, mm
I Cross sectional moment of inertia, mm4 e
I Average effective second moment of area, mm4 1
k A factor accounting for the bond characteristics 2
k A Factor related to the strain shape in a concrete member f
xiii ratio cr K Cracked stiffness, kN/mm t K Un-cracked stiffness, kN/mm f l Fibre length, mm a M Applied moment, kN.m cr M Cracking moment, kN.m n
M Ultimate moment capacity, kN.m
P Ultimate applied capacity, kN
P First crack load, kN
r Radius of fibres, mm
s Experimental average crack spacing between cracks, mm max
s Experimental maximum crack spacing between cracks, mm m
s Theoretical average crack spacing between cracks, mm
s Experimental minimum crack spacing between cracks, mm
V Fibre Volume Ratio, %
w Factor to account for concrete density
w Average crack width, mm
w Maximum crack width, mm
y Distance from centroid to extreme tension fibre, mm 0
Orientation factor of steel fibres 1
Length efficiency factor of steel fibre b
Bond efficiency factor of steel Fibres f
Fibre aspect ratio
Factor for fibre shape and concrete type
Compression steel reinforcement ratio b
Effective reinforcement ratio of conventional reinforcement
σ Stress in the tensile reinforcement calculated based on cracked section, MPa
σ Stress in tensile reinforcement under the first crack, MPa
Post cracking tensile Resistance of fibres reinforced concrete, MPa
Steel strain at stress fs
Mean strain in concrete between cracks u
Concrete strain at ultimate load
Tensile strain for fibres
Mean strain in the reinforcement
Reduction factor for lightweight concrete
ACI American concrete institute
CEB-FIP European committee for concrete
CSA Canadian standard association
EC2 European code
RILEM TC 162-TDF
Test and design methods for steel fibre reinforced concrete
The definition of high strength concrete (HSC) is always changing due to the rapid development in concrete technology. Concrete that was known in the past 50 years as high strength is considered now as low strength . In the 1950s, concrete with a compressive strength of 30 MPa was considered as high strength concrete. By the end of the 1980s, concrete with a compressive strength of 100 MPa was produced and used in some practical constructions (Rashid and Mansur, 2009). The ACI committee 211 defines HSC as concrete that possesses a specified compressive strength of 42 MPa or higher. Other codes such FIP-CIB Model Code describes HSC concrete as the concrete that has a compressive strength of 60 MPa.
In terms of its high strength, many advantages can result from using HSC compared to conventional concrete. The use of HSC would result in reduced dimensions of compressed members such as columns and piles thus increasing usable floor space. Also, the use of HSC in buildings would cause reduced both the self-weight of the structure due to the reduction in both floor thickness and supporting members sections.
High strength concrete has a steeper descending stress-strain curve compared to normal strength concrete due to the quick drop in the compressive strength in the post-
peak load region leading to brittle mode of failure (Palmquist et al., 2001). Such a problem might affect the ductility of the high strength concrete.
In addition to the compressive strength, High Strength Concrete (HSC) has excellent durability characteristics in terms, of its low permeability, absorption, chloride ion permeability (RCPT), and high abrasion resistance, which makes it suitable for use in harsh environments. Hence, HSC is also referred to as High Performance Concrete (HPC). For the past four decades, HSC has been successfully used on a commercial scale in the construction of tall buildings, long span bridges, and marine and offshore structures.
Commercial demand for lighter weight concrete has increased in recent years. This is due to its inherent economy and advantages over conventional concrete in large structures. Light weight aggregate concrete (LWAC) reduces the dead weight of the structure and the strength-to-weight ratio compared to conventional normal weight concrete is advantageous. As a result of reduced weight of structure, the inertia force is decreased in seismic regions. Moreover, the use of LWAC has become economically feasible and provides advantages for offshore structures, floating offshore structures and temporary floating ground-based structures such as liquefied natural gas (LNG) terminals.
Other advantages of LWAC are improved durability properties, fire resistance and lower thermal conductivity compared to normal weight concrete. The major disadvantage of LWAC is increased brittleness compared to normal density concrete. On the structural
level, the use of LWAC will generally result in larger cracks, deformations, and lower ductility under similar loading conditions.
Due to the considerable improvement in concrete technology in recent years, the production of high strength light weight concrete with a compressive strength of more than 70 MPa has become practically possible. ACI committee 213R considers lightweight concrete to be high strength when the compressive strength is greater than 40 MPa. To produce different levels of high strength lightweight concrete, pozzolans such as (fly ash, silica fume, metakaolin, calcined clays, and shales) are used.
The design of reinforced concrete structures should meet the ultimate and serviceability limit states criteria. The ultimate limit state requires that a structure function without damage under the normal expected loads, and under abnormal (but probable overloads), including earthquake or extreme winds, the likelihood of collapse should be minimal. The serviceability limit states requires that under expected loads the structure perform satisfactorily with regard to its intended use, without discomfort to the user due to excessive deflection, dynamic effects (vibration, acceleration), or other similar ill effects.
In addition to meeting the limit states criteria, a structural engineer should also insure that the members exhibit adequate ductility under overload conditions. Ductility refers to the ability of structural members to withstand large deformation after the yielding of tensile reinforcement. The ductility of individual structural members, as well as that of an entire structure, becomes a major design consideration in earthquake regions.
Another serviceability criterion for a satisfactory structural design is to limit the cracks that form in concrete members to an acceptable width. The definition of what is acceptable depends on the intended use of the structure, the anticipated loading, and the environment to which it is exposed. In general, for a water-retaining concrete vessel or a foundation wall protecting a dry basement space, 0.5 mm cracks that allow water to seep through are not acceptable. However, the same cracks in a non-exposed beam within a building envelope may be permissible. Engineering judgment, durability requirements and experience should lead to a decision on the level of crack control that is necessary. On the other hand, satisfying the crack width and crack spacing requirements could be the dominant governing criteria in some structures such as marine and offshore structures. Guidelines are given by codes of practice for crack width and crack spacing requirements.
The known brittleness of LWAC compared to normal density concrete has limited the use of the material. Demands for energy dissipation and/or a controlled behaviour after failure may exclude LWAC as a preferred material. In addition, the use of high strength concrete in exposed structures is required to meet durability requirements.
The addition of steel fibres to high strength normal and light weight concrete is an attractive alternative that has been found to improve the performance of concrete. The real start in studying the potential of fibres as reinforcement was performed in early 1960s. Since that time, many experimental and theoretical investigations have been conducted to study the influence of different fibre characteristics and types on the behaviour of concrete (ACI committee 544.1R-96).
At the material level, Steel fibres work by increasing the tensile and flexure strength of concrete, and improve the toughness due to the enhancement of the post-crack behaviour. Using fibres also enhances the structural performance by improving the ductility, cracking, and enhancing the fatigue performance of high-strength LWAC. By limiting crack width and thus moisture ingress, the corrosion of the reinforcement and the resulting deterioration of the concrete can be avoided (Shah, 1991).
The addition of steel fibres was found to significantly improve the mechanical properties of high strength lightweight concrete (Jianming Gao et al., 1997). Steel fibres control both cracking and deflection at service loads since they resist the growth and the widening of the cracks through the birding action mechanism (Meda et al., 2012). The addition of steel fibre to reinforced concrete beams appears to increase both flexural and shear strength (Kima et al., 2016).
Fibres are effective in improving crack development of a concrete structural element, causing a higher number of cracks and consequently lower crack spacing values and narrower crack widths compared to the concrete matrix alone. This effect can be exploited to improve the design for durability requirements of concrete structures, especially those exposed to aggressive environments.
The current Canadian Design Codes CSA A23.3-14 do not have any design provisions for steel fibre reinforced concrete. The American Concrete Institute design code ACI 318 does not have any provisions either except for allowing the use of steel fibres as minimum shear reinforcement in normal strength normal weight reinforced
concrete beams. ACI 318-14 allows the use of fibres as minimum shear reinforcement for such beams provided that the beam height is less than 600 mm, the compressive strength is less than 40 MPa and the length-to-diameter ratio of the fibres is at least 50 mm and not exceeding 100 mm.
On the other hand, the European Codes have a more active approach towards developing design provisions for crack width and spacing in steel fibre reinforced concrete structural elements. This includes the recent development of the RILEM TC 162 TDF and the new MC2010. Nonetheless, those provisos were primarily developed for normal strength normal weight concrete. Hence, further validation of these code equations and models by experimental results is still needed especially for different types of concrete.
1.2 Research Scope and Objectives
In the current research, the structural behaviour of high strength steel fibre normal and lightweight aggregate reinforced concrete beams is investigated. To achieve this objective, twelve full scale beams were cast and tested. Three different parameters were under investigation in order to develop and improve current understanding of the effect of steel fibre on the structural behaviour of high strength normal and lightweight aggregate reinforced concrete beams in flexure. These parameters were the concrete type (normal weight concrete NWC and light weight aggregate concrete LWAC), steel fibre volume ratio (0%, 0.375%, 0.75%), and flexure reinforcement ratio (0.85%, 1.50%). Three different concrete mixtures with different steel fibre volume ratios were developed and used for each type of concrete to construct the test beams. For each type of concrete,
the beams were divided into two main groups, each with different reinforcement ratios. The material proportions used to make each concrete mixture were based on different trial mixtures that were first conducted in the concrete lab at Memorial. These trial mixtures covered many different proportion of cement, water, fine aggregate, coarse aggregate, steel fibre, superplasticizer and retarder. The mechanical properties of the chosen concrete mixtures, used to cast the test beams, were evaluated by conducting several tests which including the compressive strength, splitting strength, modulus of elasticity and modulus of rupture. All beams were tested in four loading points. Test data was recorded through a data acquisition system connected to a personal computer. All obtained data and observations were analyzed and then compared to results obtained by applying different code equations and different models presented by previous researchers.
The main objectives of this study are summarized as follows;
1. To investigate the flexural behaviour of steel fibre high strength normal and lightweight aggregate reinforced concrete beams in terms of deflection, ductility, stiffness, strain, and flexural capacity.
2. To assess the serviceability performance of steel fibre high strength normal and lightweight aggregate reinforced concrete beams in terms of cracking (crack width and crack spacing) and deflection behaviour.
3. To examine the design limits of the serviceability limit states for the beams based on the obtained results.
4. To add to the experimental data bank in the literature on steel fibre high strength normal and lightweight reinforced concrete beams, in order to will assist in improving the understanding of the behaviour of such beams.
5. To validate code equations and the models proposed by different committees and researchers for high strength normal and light weight concrete beams.
1.3 Thesis Outline
Chapter 1 presents a brief introduction on the high strength concrete and an overview on the research scope, objectives and outline of this study.
Chapter 2 contains the literature review of previous work on the mechanical and flexural behaviour of high strength normal and lightweight concrete with and without steel fibres. In addition, the current codes provisions available to predict the flexural capacity, crack width and crack spacing of reinforced concrete (RC) beams are presented.
Chapter 3 presents the material proportions, standard testing and mechanical properties of the concrete used to construct the test beams for this study.
Chapter 4 describes the experimental program. Details of the test setup, preparation of test specimens. The instruments used and testing procedure are also presented.
Chapter 5 presents the results and observations obtained from the experiments. These results covers the load-deflection behaviour, concrete and steel strains, flexural capacity, mode of failure, crack width and crack spacing. In this chapter, the experimental results are also compared to the predictions obtained from the codes and expressions identified in the literature in Chapter 2.
Chapter 6 presents the summary and conclusions drawn based on the experimental observation and codes validations.
This Chapter is divided into two parts: the first part presents a brief review of mechanical properties of steel fibre reinforced concrete, followed by relevant experimental investigations and research on high strength normal weight beams and normal strength light weight concrete beams. There are no studies published in the literature on steel fibre high strength light weight aggregate concrete beams in flexure. Hence, this topic is not covered in this review. The second part of the chapter presents the current codes provisions available in the literature covering the flexural capacity, crack width and crack spacing of flexure members.
2.2Previous Experimental Investigations
2.2.1 Mechanical Properties of Steel fibre Concrete
22.214.171.124High Strength Steel Fibre Normal Weight Concrete
The effectiveness of fibre inclusion in improving of mechanical performance of high strength normal and lightweight concrete was investigated by Balendran et al. (2001). The compressive strength of the concrete was varied 90 MPa to 115 MPa. Steel fibres with volume ratio of 1 % were utilized in this study. The test results showed that cylinder splitting tensile strength and modulus of rupture improved significantly with the steel fibre. However, insignificant impact was noticed on the compressive strength. The
enhancement of splitting tensile strength and modulus of rupture was more effective for lightweight aggregate concrete compared to normal weight concrete. Toughness was also investigated based on ASTM C1018. It was observed that the toughness index of lightweight fibre reinforced concrete was not influenced by the specimen size, whereas increasing the specimen size of normal weight concrete resulted in smaller toughness index for normal weight concrete.
Song and Hwang (2004) conducted an experimental study of the mechanical properties of high strength steel fibre reinforced concrete. Four steel fibre volume ratios were applied while holding the aspect ratio constant for all mixes. The fibre volume ratio varied between 0.5 % and 2 %, whereas the aspect ratio of the fibre was chosen to be 64, with fibre length of 35 mm and fibre diameter of 0.55 mm. The compressive strength of the mixes ranged between 85 MPa to 98 MPa. It was concluded that the addition of fibres improved the compressive strength of high strength concrete and reached its maximum effect when the fibre volume ratio was 1.5 % and then started slightly decreasing with additional steel fibre. Moreover, as steel fibre increased, both the splitting tensile strength and modulus of rupture effectively improved.
126.96.36.199Normal Strength Steel Fibre Lightweight Concrete
Wang et al. (2012) conducted an experiment to evaluate the static and dynamic mechanical properties of steel fibre reinforced lightweight aggregate concrete. The study included five series of fibrous light weight concrete specimens with fibre volume ratios of 0 %, 0.5 %, 1.0 %, 1.5 %, and 2 %. For all mixes, the water cement ratio and the coarse to fine aggregate ratio were maintained consistent and equal to 0.42 and 1.3 respectively.
The addition of steel fibres was observed to slightly enhance the compressive strength of lightweight concrete. However, as the steel fibre volume ratio increased the tensile strength, flexure strength, and flexural toughness improved significantly. The impact resistance of lightweight concrete was also reported and it was evident that the usage of steel fibres improved in the impact strength. In general, the addition of steel fibres significantly improved the strength and fracture toughness of high strength light weight concrete. the authors also deduced that there was a logarithmic relationship between flexural toughness energy and impact energy of fibrous light weight concrete.
Li et al. (2016) investigated the influence of fibre content on the flexural properties of steel fibre lightweight aggregate concrete prisms. Four levels of fibre volume ratios between 0% to 2.5% were used with a constant fibre aspect ratio of 54. The maximum compressive strength reported in this study was 42.6 MPa. Based on the experimental observations, it was concluded that the workability of lightweight concrete was reduced due to the introduction of steel fibres. The addition of fibres seemed to increase the compressive strength and enhance the post cracking ductility of lightweight concrete. Moreover, the width of cracks in the aggregate-paste interface was less than the fibre-paste interface, and increasing steel fibre resulted in more voids between the fibres and the paste. Based on the findings, the authors recommended 2 % fibre content as the most effective in improving the flexural toughness of plain lightweight concrete.
188.8.131.52High Strength Steel Fibre Lightweight Concrete
Gao et al. (1997) reported and investigated the mechanical properties of fibre high strength lightweight concrete with compressive strength up to 85.4 MPa. Three steel fibre
aspect ratios of 46, 58, and 70 were used. The volume fibre ratios were 0 %, 0.6 %, 1.0 %, 1.5 %, and 2 %. The results of compressive strength, tensile strength, flexural strength, modulus of elasticity and poisson‟s ratio tests are presented and discussed. The results show that the addition of steel fibres increase the compressive strength of high strength light weight concrete. Also, a significant increase in splitting tensile and flexural strength occurred due to the bridging effect of the steel fibres. The obtained splitting tensile strength ranged from 4.95 MPa to 8.8 MPa, while the flexural strength was rated between 6.2 MPa and 11.8 MPa.
The authors presented Figure 2.1 which shows typical load versus deflection curves for steel fibre high strength lightweight concrete prism with volume fibre ratios of 1 %, and 2 % and fibre aspect ratios of 70 and 58.
A significant increase in the flexural capacity occurred due to the inclusion of steel fibres. An increase of both the fibre volume ratio and the aspect ratio caused the deformation at the ultimate load to increase with a corresponding increase in the ultimate load and flexural fracture toughness.
The effect of steel fibres on the mechanical properties of high strength lightweight aggregate concrete was investigated by Kayali et al. (2003). The tested mechanical properties included compressive strength, indirect tensile strength, modulus of rupture, modulus of elasticity, stress–strain relationship and compression toughness. A total of 8 concrete mixtures with different steel fibre content were developed. The lightweight aggregate consisted of sintered fly ash with three different sizes. All tests were carried out according to ASTM standards. The maximum compressive strength was 72.5 MPa. It was noted that a significant increase in the indirect tensile strength, the modulus of
rupture, and the compression toughness was obtained, when the steel fibres were added. However, the addition of steel fibre appeared to slightly reduce the modulus of elasticity and altered the shape of stress-strain curve to be more curvilinear.
Figure 2.1: Typical Flexural Load-Deflection Curves of Steel Fibre High Strength Lightweight Concrete (Gao et al. 1997).
2.2.2 Flexural Behaviour of High Strength Reinforced Concrete Beams
A study was carried out by Ashour et al. (1998) to investigate the effects of compressive strength and reinforcement ratio on the flexural behaviour of high-strength concrete beams. The authors investigated nine high strength concrete beams with concrete compressive strength ranging from 48 MPa to 102 MPa. Three levels of longitudinal reinforcement ratios were used. It was concluded that the load at which the first crack happened, increased due to an increase in concrete compressive strength. Moreover, the measured cracking moment was compared to the theoretical cracking moment and it was
found that American code (ACI318-98) overestimated the cracking moment of the high strength concrete beams.
The response of high strength concrete beams in flexure was also investigated by Rashid and Mansur (2005). Sixteen beams with a cross section of 250 mm × 400 mm and clear concrete cover of 20 mm were tested. The beams were simply supported over a span of 3400 mm. Four different parameters were investigated. The parameters comprised the concrete compressive strength, longitudinal reinforcement, compressive reinforcement, and stirrup spacing. The concrete compressive strength varied between 42.8 MPa and 126.2 MPa and was the main parameter in this study. To obtain more reliable conclusions, the authors considered the results obtained previously by other investigators. It was concluded that ACI318 code was able to predict the cracking moment of high strength concrete beams. Furthermore, at an assumed service load that was defined as the ultimate load divided by 1.7, the ACI318-05 code underestimated the deflection of the high strength concrete beams. It was also noted that the maximum crack width increased when the compressive strength increased. It was further reported that the ductility of the beams was obtained due to an increase in the concrete compressive strength up to 105 MPa. However, a reduction in the ductility occurred when the compressive strength passed 105 MPa.
2.2.3 Flexural Behaviour of Normal Strength Steel Fibre Reinforced Concrete
The flexural behaviour of fibre reinforced concrete beams was investigated by Oh(1992). Nine beams with steel fibre volume ratio of 0 %, 1 %, 2 % were tested. The
steel fibre had a length of 40 mm and a diameter of 0.7 mm and thus the fibre aspect ratio was consistent for all beams and equal to 57. The test beams were categorized into three series, two of which were singly reinforced beams while the third series was of doubly reinforced beams. All beams had the same dimensions of 120 mm × 180 mm × 2000 mm and they were tested under four loading points with a clear span of 1800 mm. The compressive strength of each series were 40.3 MPa, 43 MPa, and 47.8 MPa respectively. It was reported that the ultimate moment capacity increased when the steel fibre volume increased. Moreover, increasing fibre volume enhanced both the ductility and energy absorption and the effect of fibre was more evident in beams with less longitudinal reinforcement. The cracking behaviour was also investigated of this study, and it was noted that the crack width and crack spacing decreased as a result of adding more steel fibres.
The author also suggested a model by which the bending capacity of fibrous singly and doubly reinforced concrete beam can be calculated, this model was as follows:
' ' 2 2 2 t n s y s s b h c h c a a a M A f d A d (2.1)
The position of neutral axis can be calculated by equating the internal forces shown in Figure 2.2, which would result in the next formula:
' 0.85 s y t c t A f bh c f b b (2.2)
The post cracking tensile resistance of fibre reinforced concrete
tcan be calculated as follows: 0 1 2 f t b f f l d (2.3)
0 1 b are orientation factor, length efficiency factor, and bond efficiency factor of steel fibre, respectively. The orientation factor
0 and the bond efficiency factor
b are assumed to be roughly 0.41 and 1 respectively, whereas the length efficiency factor can be calculated by:
1 1 tanh 2 2 f f l l (2.4) where 2 m f f f G s E A r 25 f f f l s V d
where Gmis the shear modulus of concrete matrix, Ef is the elastic modulus, Af is the and cross-sectional area of fibre, s is the average spacing of fibre, rf is the radius of
fibre, Vf is the volume ratio of the fibre, df is the diameter of the fibre and lf is the length of fibre.
Vandewalle (2000) conducted an experimental investigation and theoretical study on the crack behaviour of normal weight concrete beams with different fibre volume ratios and different fibre aspect ratios. Five beams with a concrete compressive strength of 42 MPa and dimensions of 200 mm × 350 mm × 3600 mm were tested. Fibre volume fraction of 0.38 %and 0.56 % with two aspect ratios of, ⁄ , 65/35 and 80/50 were utilized in this study. The author concluded that at the assumed service moment, no significant difference in the crack spacing can be found as a result of changing the test parameters. However, when the load exceeded the service load, increasing the aspect ratio decreased the crack spacing. Moreover, the crack width at the service moment was reduced to about 37 % when steel fibres were used. It was also reported that the effect of changing either the aspect ratio on fibre volume ratio had no clear influence on the crack width at the assumed service load. However, when exceeding the assumed service load and at higher moment values, increasing the aspect ratio resulted in a notable reduction in the crack width. Based on the results obtained from the experiment, the author proposed an equation to predictthe crack width for hooked end steel fibre reinforced members, as presented in Eq. 2.7. This formula was constructed and improved based on the EC2-91 code formula which is recommended to predict the crack spacing for members not containing steel fibres.
m rm sm
19 Where 1 2 50 50 (50 0.25 / ) 1 ( / ) ( / ) rm b r f f s k k d with L d L d 2 1 2 1 s sr sm s s E
where srmis the average final crack spacing between cracks,
smis the mean strain in the tension reinforcement,k1is taken as 0.8 for high bond bars, k2is equal to 0.5 for a member subjected to pure moment,
sis the stress in the reinforcement calculated based on cracked section analysis,
sris the stress in the reinforcement at first crack,Esis the modulus of elasticity of the longitudinal reinforcement,
1is a coefficient taken as 1.0 for high bond bars and
2is a coefficient related to the loading duration and taken as 1.0.
The steel fibre contribution to the flexural behaviour of seven reinforced concrete beams was investigated by Meda et al. (2012). Beams behaviour at both the ultimate and serviceability limit state was the focus of the study, particularly the effect of fibres on ductility, crack width and tension stiffening. The test beams had a dimensions of 200 mm × 300 mm × 4000 mm with a clear span of 3600 mm. Beams were reinforced against shear failure with leg stirrups distributed outward from the constant moment zone at constant spacing of 100 mm. The cylinder concrete strength varied from 33.5 MPA to 45.5 MPa. Two longitudinal reinforcement ratios of 0.75 % and 1.5 % were considered. Steel fibres with constant aspect ratio of 50 were used and added to mixes in two different quantities 30 kg / m3 and 60kg / m3. All beams were tested under four point loading. The
obtained results showed that the use of fibres influenced the initial failure mode of the beams where steel fibres caused the longitudinal reinforcement to rupture instead of crushing the concrete. In addition, the increase of fibre content reduced the ductility of the beams which was attributed to the strain concentration in the steel bars. The ultimate moment did not show any significant increase due to the usage of fibres. Furthermore, fibrous beams with high longitudinal reinforcement did not undergo any sudden crushing in the concrete. the crack width and crack spacing were not investigated in the study.
Shaoo and Sharma (2014) conducted an experiment on the effect of steel fibre content on the behaviour of concrete beams with and without stirrups. Twelve reinforced concrete beams with steel fibre were tested to study both shear and flexural response under monotonic loadings. Beams had dimensions of 150 mm × 300 mm × 2100 mm over a clear span of 1800 mm. End-hooked steel fibre was used in the this study with fibre aspect ratio of 80 slenderness and volume ratio ranging between 0.0 % and 1.5 %. Three levels of reinforcement ratio were applied, these levels were 0.87 %, 1.15 %, and 1.95 %. The compressive strength of the test beams varied between 19.1 MPa and 32.9 MPa. It was concluded that flexural strength and ductility increased when steel fibres were added. However, when fibre volume fraction exceeded 0.5 %, further increase in flexural strength was not notable.
Deluce et al. (2013) proposed a new model (Eq. 2.8 and Eq. 2.9) for the calculation of crack spacing and crack width in reinforced concrete members with steel fibres. The model was developed to account for the effect of different steel fibre aspect ratios and different tensile reinforcing steel ratios. The author conducted an experimental
program on specimens subjected to direct tension. Results of crack spacing and crack width for 17 plain reinforced concrete and 53 steel fibrous specimens are compared to those predicted by the proposed models. It is concluded that the proposed models are adequate in predicting the crack spacing and crack width for fibre reinforced concrete beams. It is also claimed that the model performance is better than other currently available models. The proposed Eq. 2.8 for average crack spacing calculation was developed based on the CEB-FIP 1978 crack spacing formula.
1 2 3 2 10 b m mi s k k s c k s (2.8) , , cr avg m t avg w s (2.9) where 2 , 0.5 b 15 b p s eff d s d , s eff f f mi f p f V s k d d
3 min , 0.015 1 1 1 0.015 f f V k k 1.0 50 f f f l k d
where smis the average crack spacing, wcr avg, is the average crack width, cis the concrete cover, db is the bar diameter,
s eff, is the effective reinforcement ratio of conventional reinforcement, k3 is a fibre content factor, k1 is a factor accounting for the bond characteristics and is taken as 0.4 for deformed bars, k2 is a factor related to the strain
shape in a concrete member and is taken as 0.25 in case of uniaxial strain condition, kf
is a factor accounting for fibre effectiveness due to the fibre aspect ratio,
f is the fibre aspect ratio, lf is the fibre length and df is the fibre diameter.
2.2.4 Flexural Behaviour of High Strength Steel Fibre Reinforced Concrete beams
To account for high strength concrete, Imam et al. (1995) modified the ACI 544 equation, which was developed for predicting the flexure capacity of fibrous reinforced normal strength concrete beams. The verification of the modified ACI544 equation was done by utilizing available experimental data collected by the authors, in addition to the results obtained by testing 16 high strength reinforced concrete beams with compressive strength of 110 MPa. The modified equation was improved by changing the tensile stress of steel fibre concrete coefficient from 0.00772 to 0.002 to account for higher fibre- high strength concrete bond. This new coefficient represents bond strength of 4.15 MPa, whereas the previous coefficient of 0.00772 which is allocated for normal strength concrete represents a bond strength of 2.3 MPa. Figure 2.2 shows the simplified stress diagram along with the strain diagram of fibrous reinforced concrete section presented by the authors.
Figure 2.2: Stress and Strain Diagram of Fibrous Reinforced Concrete Section.
The modified equation suggested to calculate the nominal capacity of high strength reinforced concrete beams with a rectangular cross-section was given as follows:
2 2 1 2 0.83 0.75 2.15 2 n y M f bd Fbd (2.5) where ' 2.32 0.85 3.08 y c f F a d f F 2.0 t F
( f / f ) f f F L D V d
An experimental investigation associated with the effect of steel fibre on the shear resistance of reinforced concrete beams was conducted by Khuntia et al (1999). The next
simplified formula (2.6) was suggested by the authors to be used to calculate the post cracking tensile resistance of steel fibre reinforced concrete
' 0.28 t F fc (2.6) Where f f f l F v d
is the shape factor which is assumed to be 1 for normal weight concrete, and vf
is the volume of fibre in percentage.
Chunxiang et al. (1998) conducted an experiment to evaluate the properties of high-strength steel fibre reinforced concrete beams in bending. Ten beams were fabricated and cast with concrete that had a compressive strength fluctuating between 72.8 MPa to 92.2 MPa. The cross section of the beams was selected to be 120 mm × 150 mm whereas the support length for the beams was 2000 mm. Three different fibre aspect ratios were investigated. The fibre volume ratio was 1 %. The aspect ratios were 38, 45, and 46. Three of the beams were reference specimen without fibres. The authors concluded that the flexural rigidity of the beams increased before the yielding stage due to the addition of steel fibres. Furthermore, the increase in the rigidity mainly depended on the fibre aspect ratios, where the smaller fibre resulted in improving stiffness of the beams. It was also concluded that the displacement of the fibrous beams at failure increased compared to the reference beams.
A study of flexural cracking behaviour of normal strength, and high strength steel fibre concrete beams, using the Digital Image Correlation technique was conducted by Harmrat et al. (2015). The study focused on the crack behaviour of different normal weight concrete types. The authors also evaluated the accuracy of different codes in evaluating the crack width. Nine beams were divided into three groups based on the compressive strength and fibre content. Group one comprised three normal strength concrete beams with a compressive strength of 44 MPa. Group two had three fibre reinforced beams with a high compressive strength of 78 MPa, whereas group three consisted of three beams with high a compressive strength of 85 MPa. Steel fibre with a length of 40mm and an aspect ratio of 80 was added to the mix that was used to cast the second group with steel volume ratio of 0.5 %. Three longitudinal reinforcement areas were used for each group, those areas were 157 2
mm , 226 2
mm , and 308 2
mm . It was concluded that the addition of steel fibres increased the first cracking load by 10 % to 25 % of the ultimate load. Furthermore, a reduction of 35 % to 70 % occurred in final average crack spacing and crack width at assumed service load. The beams were 100 mm × 160 mm × 1500 mm, tested using four points loading over a span of 1300 mm. It was also noted that predicting crack width using BS8110 and Eurocode EC2-04 formulas was found to be acceptable for all beams without steel fibre.. The beams tested in the study are more representative of a material level than a structural one due to the small depth of the specimen. Moreover, there appears to be an error in the load versus crack width plots as they used the actuator load rather than the support reaction. Good predictions were
obtained when applying RILEM TC-162-TDF crack width model to fibrous concrete beams.
2.2.5 The Flexural Behaviour of Normal Strength Reinforced Lightweight
Wu et al. (2011) tested six beams to study the flexural behaviour and size effect of lightweight aggregate concrete beams. The longitudinal reinforced ratio varied between 0.33% to 1.3%. Beams were fabricated and cast with different dimensions and constant concrete compressive strength of 34 MPa. Six beams were tested. Beams had a depth that varied from 400 mm to 700 mm. It was concluded that lightweight concrete beams exhibited similar flexural capacity to their corresponding normal weight concrete beams. Nonetheless, lightweight concrete beams displayed higher deflection compared to normal weight concrete beams. The test results revealed that increasing the depth of the beams from 400 mm to 700 mm resulted in a decrease in the ultimate capacity ratio. That indicates a size effect due to the increase in the beam depth. Moreover, the authors compared the experimental deflection at assumed service load to that calculated using ACI 318 code and indicated that the ACI 318 code underestimates the service deflection for both normal and lightweight concrete.
2.2.6 The Flexural Behaviour of High Strength Reinforced Lightweight Concrete
The flexural behaviour of reinforced high strength lightweight concrete beams was investigated by Shuaib and Baker (1991). This study was performed by testing six singly reinforced beams over a length of 3.45 m. The compressive strength of the beams
varied between 39.9 MPa to 75.9 MPa, and the longitudinal reinforcement ratio to balanced reinforcement ratio
/ b, ranged from 0.18 to 0.54. All beams were 152.4 mm wide and 304.8 mm deep, the effective depth varied between 228.4 mm and 260.4 mm. It was concluded that for low reinforcement ratio , which was between 0.01 to 0.025, increasing
caused a notable reduction in the displacement ductility. However, after exceeding reinforcement ratio of 0.025, the displacement ductility continued to slightly decrease until it became insignificant at higher levels of reinforcement. It was also noted that for reinforcement steel ratio
/ bless than 0.5, the increase in compressive strength decreased the displacement ductility index. Moreover, beams with a compressive strength of 75.9 MPa displayed insufficient ductility of less than three, when the reinforcement ratio
/ bwas 0.24. The author also compared the ultimate moment capacity obtained experimentally to that predicted using the ACI318 code. It was concluded that the code gave a conservative prediction of the ultimate flexural capacity for the lightweight concrete beams with compressive strength not exceeding 75.9 MPa and
/ bnot greater than 0.54. It was also found that the strain value of 0.003 recommended by the ACI318 code seemed to be acceptable for high strength lightweight concrete with a compressive strength less than 75.9 MPa.
Shuaib and Batts (1991) conducted an experiment to evaluate the flexural behaviour of doubly reinforced high-strength lightweight concrete beams with web reinforcement. Two main variables were investigated in this study, compressive strength and the longitudinal reinforcement ratio to balanced reinforcement ratio,
/ b. The
compressive strength varied between 46.2 MPa to 76.3 MPa, whereas the tensile steel ratio,
/ b ranged between 0.16 to 0.47. Six doubly reinforced beams with a cross section of 152.4 mm × 304.8 mm and a length of 3.6 m were investigated. It was concluded that when increasing the compressive strength, the displacement ductility index decreased. However, after the
/ bratio exceeded 0.22, it seemed that the compressive strength had no influence on the ductility. It was further reported that the ACI318 rectangular stress block underestimated the flexural capacity for high strength lightweight concrete beams. Hence, it was considered safe to estimate the flexural capacity using ACI318 code. Ultimate compressive strain in the concrete was also investigated. The obtained results indicated that the strain of 0.003 recommended by ACI318 code seemed to be acceptable for doubly reinforced high strength lightweight concrete beams with compressive strength not exceeding 75.9 MPa.
The flexural behaviour of lightweight aggregate concrete (LWAC) beams was investigated by Sin (2011). Eighteen beams with dimensions of 150 mm × 300 mm × 3100 mm were tested. The beams were simply supported over a span of 2.8 m. Three normal weight concrete (NWC) beams were added as reference specimen . Five parameters were examined and the test beams were categorized into five groups. Only one parameter was changed at a time, whereas all other parameters were kept constant. The vareid parameters were compressive strength, longitudinal reinforcement in compression and tension zone, transverse reinforcement and total perimeter of flexural reinforcement. The compressive strength varied from 20 MPA to 80 MPa, whereas the reinforced steel ratios were 0.67 %, 1.02 %, 1.45 %, 1.61 % and 2.22 %. Four levels of
compression reinforcement ratio were used, these levels were 0 %, 0.43 %, 0.73 %, and 1.11 %. In the flexure zone, the authors varied the amount of transverse reinforcement in order to investigate their effect of the confinement of the compression reinforcement on the beams ductility. The spacing between the stirrups ranged from 50 mm to 180 mm. Three different bars with diameters of 13 mm, 16 mm, and 20 mm were used. It was observed that all beams failed in flexure mode where the steel yielded first followed by crushing of the concrete zone.
The authors concluded that the number of cracks of LWAC beams at the assumed service load was higher than the number of cracks in the identical NWC beams. The assumed service load was defined as the ultimate load divided by 1.6. It was also noted that the maximum crack width in LWAC beams is less than that in NWC beams. The deflection of the LWAC beams in comparison with LWAC beams was also studied. It was found that the LWAC beams had higher deflection compared to the NWC beams. However, the test results reveals that LWAC beam with compressive strength of 79 MPa had 9 % lower deflection than its corresponding NWC beams. The moment capacity of the LWAC beams appeared to be identical to the NWC beams. However, LWAC beams showed less curvature ductility than NWC beams.
A study was conducted by Almousawi (2011) to evaluate lightweight concrete beams in flexure. The author tested fourteen lightweight beams with a cross section of 200 mm × 300 mm, and with a length of 3600 mm. Three different parameters were investigated; the compressive strength, flexural reinforcement ratio, and compression steel reinforcement ratio. The concrete compressive strength varied between 50.9 MPa to 68.5 MPa. The conclusion was that the ultimate load capacity of beams increased as a
result of increasing the compressive strength. Moreover, increasing either longitudinal tensile reinforcement ratio, , or compression reinforcement ratio, , resulted in an increase in the ultimate load. The displacement ductility of the beams was also measured It was found that, contrary to the increase in the compression steel reinforcement ratio, the increase in either compressive strength or tensile reinforcement ratio led to a decrease in the ductility of the beams.
Carmo et al. (2012) investigated and reported the influence of both concrete strength and transverse confinement on bending behaviour of reinforced LWAC beams in terms of strength and ductility. The study focused on three issues, mainly on the theoretical pure bending area, and partially on the cracking stage and the plastic stage. The authors tested thirteen LWAC beams with dimension of 120 mm × 270 mm × 3000 mm, these beams were simply supported over a length of 2800 mm. Beams were divided into three different groups in order to investigate the influence of each parameter. The first group was established to study the effect of varying the tensile reinforcement ratio, which was varied between 0.55 % and 2.96 %. The second group was to study the influence of the transverse reinforcement ratio Asw /s at the constant moment zone, this group was composed from six beams. Three different transverse reinforcement ratios
A s of 0 %, 0.6 % and 1.68 % were used. The third group that consisted of six beams was used to study the effect of compressive strength, which was varied from 35 MPa to 70 MPa. All beams were failed under bending. It was reported that the ability of LWAC beams to undergo deformation depends on the tensile reinforcement ratio. When increasing the reinforcement ratio, the deformation capacity would decrease.
Furthermore, the increase of compressive strength resulted in an increase in the vertical deformation in addition to increasing curvature specifically when the steel ratio was low. Within the constant moment zone and when there was no transverse reinforcement, the beams exhibited a brittle failure compared to beams with transverse reinforcement particularly for the beams with higher longitudinal tensile reinforcement ratio. It was also found that an increase in compressive strength controlled the mode of failure and changed the mode to tension failure in some cases where the beams were over-reinforced. The stiffness ratio EI /EII and ductility were measured and it was found that the stiffness ratio EI /EII was less than 2 and different from the value estimated by EC2-04 code.
2.2.7 Flexural behaviour of Normal Strength Steel Fibre Reinforced Lightweight
Altun and Aktas (2013) carried out an experiment investigation of fibre on the behaviour of lightweight concrete beams. A total of eighteen beams with dimensions of 300 mm × 300 mm × 2000 mm were tested. Beams were labeled into three series based on the cement content. Each series had three different samples and each sample was repeated twice; in total, each series had six beams. The cement dosages were 350kg/m3, 400kg/m3, and 450kg/m3, and the maximum and minimum compressive strength were 23.75 MPa and 15.5 MPa respectively. The steel fibres were 60 mm in length, 0. 75 mm in diameter with an aspect ratio of 80 and tensile strength of 1050N/mm .2 Steel fibre content ratios for each group were 0 kg/m3, 30 kg/m3, 60kg/m3.The longitudinal reinforcement area was constant for all beams and equal to 400mm2. To ensure that the